Recent progress of Ga-based liquid metals in catalysis

Within the last decade, the application of gallium-based liquid metals in catalysis has received great attention from around the world. This article provides an overview concerning Ga-based liquid metals (LMs) in energy and environmental applications, such as the catalytic synthesis of ethylene by non-petroleum routes via Pd–Ga liquid catalysts, alkane dehydrogenation via Pd–Ga or Pt–Ga catalysts, CO2 hydrogenation to methanol via Ni Ga or Pd/Ga2O3 catalysts, and catalytic degradation of CO2via EGaIn liquid metal catalysts below 500 °C, where Ga-based liquid metal catalysts exhibit high selectivity and low energy consumption. The formation of isolated metal sites in a liquid metal matrix allows the integration of several characteristics of multiphase catalysis (particularly the operational friendliness of product separation procedures) with those of homogeneous catalysis. In the end, this article sheds light on future prospects, opportunities, and challenges of liquid metal catalysis.


Introduction
Typically, liquid metal catalysts are utilized in reactions where the reaction temperature exceeds the catalyst's melting point. Several metals with low melting points including gallium (Ga), mercury (Hg), cesium (Cs), rubidium (Rb), and francium (Fr) have been favored by researchers. As the most widely studied liquid metals, Ga and Ga-based liquid metal alloys have been considered as a new class of composite materials in many elds.
While retaining the excellent electrical and thermal conductivity of conventional metals, liquid metal is the soest of all conductive substances. 1 In contrast to Hg, a common liquid metal whose toxicity limits its research and applications, the biocompatibility and near-zero vapor pressure of Ga and Gabased liquid metal alloys make Ga-based liquid metals promising for research in a variety of elds. 2 As a liquid phase metal, Ga functions as a metal solvent, and the proportions of different metals associated with Ga metal can be adjusted to create alloys with varying melting points. Gallium-Indium alloys (EGaIn) and Gallium-Indium-Tin alloys (Galinstan) are two commonly used liquid metals based on Ga. [3][4][5] The Xi Sun received his Bachelor's degree in Environmental Science and Engineering from Liaoning Technical University, and is now working on liquid metal alloy catalyst performance evaluation, advanced catalysis materials, green hydrogen, methane/ ammonia production, and high purity hydrogen separation and compression.
Professor Hui Li received his PhD in Industrial Catalysis from University of Chinese Academy of Sciences. He was awarded an Outstanding Overseas Youths award and has long been engaged in basic research on the application of palladium membrane purication materials in fuel cell hydrogen sources and large-scale hydrogen purication, and catalytic carbon conversion to highervalue products. As the project leader, he has led 10 projects, including the EU 6th and 7th framework studies, and achieved the rst industrial-scale demonstration of ultra-pure hydrogen purication (800 nm3 h À1 ) and a methane reforming palladium membrane reactor for IGCC. melting points of these two alloys (z11 C, zÀ19 C) are even lower than pure Ga (29.78 C). 4 A bimetallic or even polymetallic catalyst has greater catalytic activity than its monometallic counterpart due to the synergistic effect. 6 Liquid metals composed of Ga tend to oxidize since Ga in contact with oxygen (O) forms a nanometer-thick layer of dense, smooth metal oxide on the surface of the metal, which is partially passivated and prevents further oxidation of the metal from inside. 7 Using electrochemical methods, it is possible to manipulate the oxide species on the surface by adjusting the composition of the liquid metal or by regulating the gain or loss of electrons. 8 Under the protection of Ga, this property enables numerous active metal catalysts to increase their catalytic activity. 9 This article reviews main research advancements in Ga-based liquid metal applications in energy and environmental catalysis elds, and shed light on opportunities and challenges for future developments.
2 Categories, synthesis and fabrication

Ga-Pd bimetallic catalysts
It is possible to modify the catalytic properties of LM by dissolving noble metals or transition metals to form intermetallic compounds. Modifying the electronic structure of supported LM catalysts can alter their catalytic properties. Gallium-palladium (Ga-Pd) bimetallic catalysts are superior liquid catalysts when compared to Pd or Ga catalysts alone. According to Fig. 1(a), GaPd, GaPd 2 , and Ga 7 Pd 3 have good crystal structures, exhibiting superior electronic properties compared to the pure metal, thereby enhancing the catalytic selectivity, long-term operational stability, and catalytic performance of these catalysts in reduction or oxidation reactions. 10 Ga-Pd nanoparticles were synthesized in an inert atmosphere by dissolving palladium acetylacetonate (Pd (acac) 2 ) in tetrahydrofuran (THF) with heating and stirring, dissolving gallium trichloride (GaCl 3 ) in lithium triethyl borohydride (LiHBEt 3 ) and then pumping it into the THF solution to produce a black suspension, with prolonged stirring of the suspension. Then a centrifuge was used to separate the solid from the liquid. Aer the separation and three repeated THF rinses, the black solid sediment was extracted and dried. To ensure the formation of intermetallic compounds, the dried precipitate particles were re-dissolved in dioctyl ether for four hours with heating and stirring, and the washing and drying processes were repeated aer solid-liquid separation. 11,12

Ga-Pt bimetallic catalysts
In the hydrogenation catalytic reactions, Pt catalysts get reduced to electron decent Pt species, 13 the inclusion of gallium creates Pt-Ga assemblies such as gallium-Pt alloys on the catalyst surface, with Pt-Ga interactions. Previous work has demonstrated that iron, tin, and germanium successfully boosted the catalytic performance of Pt catalysts. [14][15][16][17] The addition of gallium signicantly increases the dispersion of platinum 18 and exhibits increased exposure of platinum active sites on the catalyst surface to the reaction atmosphere. The platinum-gallium interaction also changes the electronic structure around the platinum atom and alters the electronic properties of the platinum active center, 19 with implications for properties such as the selectivity of the Pt catalyst. 20,21 The electrocoupling substitution method can be used to prepare Ga-Pt SCALM catalysts [13] . First, pure Ga was heated and stirred in an isopropanol solvent to form a Ga suspension. Next, an aqueous solution of chloroplatinic acid was added to the Ga suspension, which was obtained through evaporation and calcination. Platinum acetylacetonate (Pt (acac) 2 ) was added to a toluene solution, evaporated from the toluene at 453 K, and calcined at 923 K for three hours in air, according to a second method. In situ XRD or catalytic measurements are capable of reducing the resulting catalyst to form Pt monometallic and/or Pt-Ga bimetallic nanoparticles on its surface. 22

Ga-Ni bimetallic catalysts
Nickel nitrate hexahydrate (Ni(NO 3 ) 2 $6H 2 O) and Ga metal were utilized to create Ni-Ga catalysts by means of stepwise evaporation co-condensation (sol-gel method) and reux cocondensation techniques. The method of preparation was as follows. Ga metal was completely dissolved in a nitric acid solution to produce Ga(NO 3 ) 3 . The acid mixture was neutralized and precipitated in excess with a concentrated NaOH solution until its pH ranged from 9.5 to 10. Utilizing a heater for 24 hours, the temperature of the mixture was increased to a range of temperatures. Aer 24 hours, the process was to gradually evaporate the water by removing the reux system, and the mixture was in gel form. The gel was washed and ltered until its pH became neutral and it solidied into a moist substance. The product was dried overnight at 100 C, followed by a six-hour calcination process at 500 C to produce white powders and calcined samples. By adding calcined samples to a NaBH 4 solution in anhydrous ethanol, the mixed oxides of Ni 2+ and Ga 3+ were converted into Ni-Ga alloys with different Ni/Ga molar ratios. 23 Alternatively, the urea hydrolysis hydrothermal method was used to fabricate the Ni 5 Ga 3 catalyst by preparing a hydrogenlike compound (HTlc) precursor with 65% nickel atom and gallium equilibrium. Ni(NO 3 ) 2 -6H 2 O and Ga(NO 3 ) 3 -9H 2 O were dissolved in 50 mL of distilled water at 65-35% molar percentages, and urea in the same nitrate ratio was then dissolved in the aqueous solution under strong stirring. Different samples of the prepared mixture were sealed in a hydrothermal reactor at 90 C, 110 C, 130 C and 150 C to study the effect of synthesis temperature. The products were maintained for 16 h, followed by centrifugation, washing with deionized water and drying at 100 C overnight to obtain the HTlc precursor. The dry cake x-HTlc produced above was crushed and sieved with 40-60 mesh, and the collected sample was reduced in a tube furnace at a heating rate of 5 C min À1 in a mixture of 5% H 2 and Ar at an equilibrium temperature of 40 mL min À1 for 6 h. The corresponding reduced metal alloy was denoted as x-Ni 5 Ga 3 . 24

EGaIn and Galinstan liquid metal catalysts
Gallium readily alloys with many metals. 25 Therefore, as a component, gallium can potentially serve to form a variety of low melting point alloys with other metals, including indium (In), 26 lead (Pb), 27 bismuth (Bi), tin (Sn), 28 aluminum (Al), zinc (Zn), 29 etc. The melting point of alloys varies depending on the composition and ratio.
EGaIn and Galinstan are metals with melting points below or close to room temperature. The EGaIn alloy was produced by combining Ga and In in stoichiometric proportions (75.5 wt% Ga and 24.5 wt% In). 30 The constituent metals were mixed in a thermoset on a heating plate at approximately 200 C (above the melting point of iron) until completely dissolved and thoroughly combined, and the alloy was allowed to cool naturally. 31 Similarly, the GaSnIn alloy was produced by melting 68.5 wt% Ga, 21.5 wt% In and 10 wt% Sn 30 in a heated beaker, stirring thoroughly, and then cooling the metal. 32 Liquid metals as such could even be dispersed into nanoparticles towards multiple functions, as can be done by a simple sonication method in the presence of organic solvents. 33 First, a certain quantity of liquid metal bulk in a vessel containing thiol ethanol solution is added and an ultrasonic probe is applied to introduce cavitation in the solution, and the liquid metal bulk stabilized by the oxide layer is rapidly fractured into numerous liquid metal nanoparticles by oscillatory shear force. This results in local extremes of pressure and temperature in an ultrashort period of time. In this case, thiolated ligands can be assembled easily and rmly on the surface of nascent liquid metal nanoparticles at the same time, competing with the oxidation process of liquid metal. Eventually, spherical liquid metal nanoparticles are formed under continuous sonication and are stabilized due to the protection of thiol ligands and the rapid oxidation of the surface. 34,35 2.5 Liquid metal/metal oxides (LM/MO) framework and Au/ Ag-Galinstan liquid metal framework catalysts Solid metal/metal oxide (SM/MO) are of tremendous interest due to their unique physicochemical characteristics of its micro-and nanostructures. [36][37][38][39] Comparing to SM/MO, LM/MO exhibits additional dimensions to the structure, with the exibility, the possibility of mixing with other metals and their recyclability, uidity, and high conformation. 40 Liquid metal framework, which consists of solid metal nanoparticles (primarily precious or transition metal species) encased in a liquid metal framework, augments the catalytic activity of solid catalysts. 41 The Au/Ag-Galinstan catalysts were synthesized using a galvanic replacement reaction. For 72 h, droplets of Galinstan were immersed in 0.1-5 mM aqueous solutions of varying concentrations of AgNO 3 or KAuBr 4 , or in 0.1-1 mM aqueous solution of KAuCl 4 . The Ag-Galinstan material was prepared by adding 80 mg of Galinstan alloy to 4.9 ml of 5 mM AgNO 3 aqueous solution, sonicating for 30 min, and then adding 0.1 ml of 5 mg ml À1 PVP. The Au-Galinstan material was prepared by sonicating 200 mg of Galinstan in 5 ml of 1 mM KAuBr 4 $xH 2 O aqueous solution for 30 min. The material that had been prepared was to be deionized. 42

Supported catalytically active liquid metal solution (SCALMS) containing single atom catalysts (SACs)
Atomically dispersed metal catalysts have attracted great interest in catalysis owing to its unique properties. Isolated single or minor metal atoms can be anchored to the substrate by chemical bonding or spatial connement to maximize the efficiency of atom utilization. Due to the near 100% availability of active atoms and the tunable microenvironment of the metal catalyst core, single-atom catalysts (SACs) have distinguished themselves in various catalytic elds with respect to enhanced rates, conversions and selectivity of industrial reactions. [43][44][45][46][47][48][49][50][51][52] As the majority of catalytic reactions take place on the catalyst metal surface, 53 the atoms of metal that are unable to reach the reactant molecules are largely wasted. 54 Noble metals (e.g. Platinum group of metals) tend to be used as superior catalysts, but with their high price and limited quantities, the proportion of these metal atoms that have no catalytically active role should be minimized. 55-57 Therefore, it is essential to explore ways to reduce the amount of precious metals used, to improve their catalytic activity and selectivity, and to increase their catalytic lifetime. 48 Employing relatively small metal particles 58 with a high surface/ volume ratio and loading on specic high area support is a common solution to the above problems. For the prevention of aggregation of metal nanoparticles during catalyst synthesis or catalytic reactions, metal nanoparticles are usually dispersed into quasi-two-dimensional shapes, like immobilized on a carrier with a high specic surface area, so that the reaction molecules can reach as many metal surface atoms as possible.
Gallium, EGaIn, Galinstan in liquid state, as metal solvent, can dissolve different metals or metal salts with different solubilities, forming a single atom catalyst layer of catalytically active metal exposed to a liquid metal surface, its liquidity enables the metal atoms on the surface to ow inwards and outwards, replacing deactivated active sites with a cycle of fresh active sites, further extending the lifetime of the catalyst while expanding the contact area between the catalyst and the reactant molecules.
Platinum powder or nanoparticles in an inert gas atmosphere (in the case of the generation of oxidation layers) can be mechanically integrated with liquid metal Ga or Ga alloys (EGaIn or Galinstan) with no Pt-Pt bonding or Pt clustering observed. 59 Unique properties determine the formation of Pt SAC. There is a solubility range for virtually all precious metals and transition metals in liquid Ga. The solubility of Pt in Ga is governed by the following equation: 60 where C is the Pt concentration in liquid Ga (at%), A ¼ 3.3 and B ¼ 2.450 are the solubility constants, and T is the absolute temperature.

Application of Ga-based liquid metals in the energy industry
The rapid development of industry has caused severe damage to the natural environment, and corresponding research has been conducted on clean energy as an alternative to traditional energy sources. Ga-based liquid metal catalysts require less energy (room temperature or relatively low temperature) than conventional thermal catalysts, 61 making them an attractive catalyst for environmental protection and clean energy applications. The formation of isolated metal sites in a liquid metal matrix permits the integration of several characteristics of multiphase catalysis (particularly the operational friendliness of product separation procedures) with those of homogeneous catalysis, as the metal sites exhibit different electronic properties due to interactions between the metals. 62 Ga-Pd liquid metal catalysts are more selective than bulk Pd catalysts in the steam reforming of methanol to hydrogen. 63

Synthesis of ethylene by non-petroleum routes
The investigation of non-petroleum ethylene synthesis routes has been a top research priority. Conventional thermal catalysis of ethylene frequently necessitates temperatures above 200 C and gas pressures of 5 bars with a high hydrogen consumption, exposing the disadvantage of high production costs. 64 Armbrüster et al. 11,12 prepared ionic metal precursors by co-reduction in tetrahydrofuran (THF) with lithium triethyl borohydride (LiHBEt 3 ) to prepare three types of crystal structures of singlephase Ga-Pd nanoparticles (GaPd, GaPd 2 , Ga 7 Pd 3 ). 10

Alkanes to hydrogen
Catalytic hydrogen production from alkanes is a widely used method for hydrogen production due to its easy product separation and mature technology. However, alkane hydrogen production is part of the gray hydrogen industry, and its byproduct CO 2 emissions cause irreparable environmental damage. Taccardi et al. 65 reported a catalytically active liquid metal solution (Ga-Pd SCALMS, Ga/Pd ¼ 1-52) loaded on porous glass with various crystal structures 10 to test the selectivity and catalytic activity pattern in butane deep dehydrogenation (BDH). Ga/Pd ¼ 52 (molar ratio) yields the best selectivity and activity towards butane. Raman et al. 66 studied a Ga-Pt based liquid metal solution (Ga-Pt SCALMS) for propane dehydrogenation (PDH) loaded on a porous carrier material at temperatures between 500 C and 600 C. The performance of liquid metal solution was compared to that of silicon dioxide (SiO 2 ), aluminum oxide (Al 2 O 3 ), and silicon carbide (SiC). It was discovered that the SCALMS loaded on the Al 2 O 3 carrier exhibited signicant scorch deactivation; the SCALMS loaded on SiC exhibited the best catalytic activity; and the SCALMS loaded on SiO 2 exhibited the highest stability and lowest tendency for cracking at higher temperatures, maintaining a propane selectivity of over 93% at 600 C. Comparing SCALMS catalysts with Pt-solid-phase catalysts and Ga-Pt-solid-phase catalysts loaded on three carriers (Fig. 2), it was discovered that SCALMS loaded on SiC demonstrated the highest catalytic activity and resistance to coking loss. Redekop et al. 22 compared the selectivity of Pt-Ga catalysts with Pt-(Mg/Al/Ga)Ox for deep propane dehydrogenation and found that Ga-containing catalysts with Ga/Pt ratios greater than 2 were less active during the initial stages of propane dehydrogenation but more selective and less susceptible to coking than Ga-free and less Gacontaining catalysts.

Carbon dioxide to methanol
Methanol from carbon dioxide hydrogenation is a method for utilizing carbon dioxide as a resource, and the product can be used for various purposes, including liquid fuel for methanol fuel cells (DMFC) and hydrogen from methanol steam reforming. Studt 67 prepared a nickel-gallium (Ni-Ga) catalyst to hydrogenate carbon dioxide to methanol at ambient pressure; the catalyst exhibited intriguing activity, selectivity, and stability for ambient pressure CO 2 reduction. The issue of carbon monoxide byproducts resulting from the reversible water-gas reaction has been resolved, and a low-pressure mini apparatus for preparing methanol from carbon dioxide has been proposed. On the basis of previous research, Nguyen et al. 23 investigated the effect of Ni-Ga catalyst preparation method, alloy composition ratio, and reaction temperature on the activity and stability of Ni-Ga catalysts with a focus on catalyst structure using a variety of instrumental techniques (XRD, STEM, TG-DTA, BET, XPS) to provide catalytic process overview. Men et al. 24 prepared HTlc precursors with 65% Ni atomic percentage and gallium equilibrium using the urea hydrolysis hydrothermal method, fabricated Ni 5 Ga 3 catalysts synthesized from hydrotalc-like compounds (HTlc) precursors for CO 2 hydrogenation to methanol, and fully characterized them. The improved catalytic performance was proven by endurance tests with constant CO 2 conversion and 100% methanol selectivity at 200 C and 0.27 s À1 turnover frequency.
Fujitani et al. 68 observed that the support had a signicant effect on the catalytic activity of the Pd-based catalysts for the synthesis of methanol from CO 2 and hydrogen, with Pd/Ga 2 O 3 showing a 2-fold higher yield and a 20-fold higher turnover frequency than Cu/ZnO, Collins et al. 69 studied the effect of palladium-gallium interactions in Pd (1wt%)/b-Ga 2 O 3 during the hydrogenation of CO 2 to methanol and made a comparison with Pd/SiO 2 and pure b-Ga 2 O 3 to characterize the catalyst material (Fig. 3). They discovered that Ga-Pd bimetallic microcrystals act to supply atomic hydrogen to the oxidation surface through spillover and inhibit the decomposition of methanol and carbon monoxide generation. At 3 MPa and 523 K, the Pd (1wt%)/b-Ga 2 O 3 catalyst reaches a 52% methanol selectivity compared to the 12% methanol selectivity for Pd (2wt%)/SiO 2 .

Methanol steam reforming to hydrogen
Methanol steam reforming manifests a relatively mild reaction condition, with an easy separation of the product and technically mature hydrogen production; the carbon dioxide in the product can be recycled in a special process to achieve zero carbon emissions when methanol is reformed with steam. Thus MSR is a highly promising process for the production of automotive hydrogen in fuel cell vehicles. 70 Li et al. 71 fabricated a series of gallia-supported Pd-Ga catalysts that consist of metallic nanoparticles on three porous polymorphs of Ga 2 O 3 (a-, b-, and g-Ga 2 O 3 ) by a controlled co-precipitation of Pd and Ga. A signicant effect of gallium polymorphs can be observed and the selectivity increases in the order of g-Ga 2 O 3 (20%) < a-Ga 2 O 3 (30%) < b-Ga 2 O 3 (40%). Lorenz 72 investigated the CO 2 selectivity of Pd-Ga 2 O 3 catalysts (Ga 2 O 3 -supported Pd-based intermetallic phases) in methanol steam reforming and tested the catalytic performance of a-Ga 2 O 3 , b-Ga 2 O 3 and g-Ga 2 O 3 crystalline forms as palladium oxide carriers in methanol steam reforming. Pd/b-Ga 2 O 3 and Pd/g-Ga 2 O 3 appear to be similarly unselective, but Pd/a-Ga 2 O 3 exhibits 85% CO 2 selectivity at 673 K (Table 1).

Application of Ga-based liquid metals in the environmental industry
Carbon dioxide, the most prevalent exhaust gas from the chemical industry, is also one of the most signicant greenhouse gases in the Earth's atmosphere, contributing up to 25% to global warming. Thus, controlling carbon dioxide emissions from industrial sources is a crucial aspect of controlling greenhouse gases. 73 Reducing and capturing carbon dioxide and methane emissions is the key to combating global warming, 74 and carbon capture, utilization and storage (CCUS) has been studied for more than a decade.

Catalytic degradation of carbon dioxide
Conventional thermal catalysis of CO 2 necessitates a substantial amount of energy while suffering from the drawbacks of catalyst deactivation and oxidation. Using Ga-In liquid metal (EGaIn) and the carbon dioxide solvent dimethylformamide (DMF), Zuraiqi et al. 75 designed a reactor for the catalytic degradation of carbon dioxide. The reduction product was either singlet carbon or carbon monoxide, and catalyst coking deactivation did not occur between 25 C and 500 C. Analysis of the catalytic products and yields (Fig. 4(a and b)) as well as the catalyst prior to and aer the reaction revealed that Ga in the alloy was the catalytically active material for the degradation of CO 2 and that Ga could regain catalytic activity through the reduction process aer being oxidized.
Esralzadeh et al. 76 added 3 wt% cerium (cerium has a solubility of 0.1-0.5 wt% in Galinstan alloys) to the Galinstan alloy to form a layer of cerium oxide on the surface of the liquid metal to degrade CO 2 (Fig. 4(e)). The solid product composition was analyzed by XPS (Fig. 4(c)), and the Faraday efficiency was calculated. The product was determined at various potentials ( Fig. 4(d)); the surface properties of the liquid metal prevented coking deactivation; the reduction of the catalyst was accomplished by applying a very low cerium reduction potential, balancing the high selectivity of the catalyst with the low energy requirement.
Tang et al. 77 utilized a suspension of Ga and Ag(I) as the precursors of the co-catalysts in a bubbling column reactor lled with dimethylformamide (DMF) and ethanolamine (ETA) with external ultrasonic and mechanical stirring and subjected to catalytic degradation of CO 2 at close to room temperature. In a reactor with a specic height and volume, up to 92% of 8SCCM CO 2 was converted into singlet carbon, oxygen, and gallium oxide (Fig. 5). The total reaction was as follows: Ga + CO 2 / Ga + + CO 2 À (1) The addition of silver ions permits the reduction of oxidized Ga to catalytically active Ga monomers via the following pathway: 4Ga + + 4Ag 0.72 Ga 0.28 / 4Ga + 4Ag 0.72 Ga 0.28 4Ag 0.72 Ga 0.28 + + 4e À / 4Ag 0.72 Ga 0.28 (6) Due to the density difference between carbon and metallic compounds, carbon sheets naturally oat on the reactor's surface. The operational costs of CO 2 capture and conversion using DMF + ETA are lower than those of any other state-of-theart technology, according to general estimates based on current electricity costs.

Catalytic degradation of organic methylene blue in wastewater
Methylene blue (MB) is a biotoxic, teratogenic, carcinogenic, and mutagenic organic cationic dye that is frequently found in Ethylene selectivity 74%-77%.  the wastewater of the printing and dyeing industries. Oen, MB-contaminated waters have a high chromaticity and abundant chemical oxygen demand (COD). Hoshyargar et al. 42 prepared a liquid metal core/solid metal shell Au/Ag-GalnSn nanoparticle for the electrical replacement of Galinstan using gold (Au) and silver (Ag). The nanoparticles' catalytic activity against MB in the presence of sodium borohydride was evaluated (Fig. 6). During contact with the reduction medium, the morphology of the Au-Galinstan catalyst changed to micron-sized spherical particles decorated with Ag nanoparticles, whereas the morphology of the Ag-Galinstan catalyst remained unchanged. The composition of the catalyst also changed, with a signicantly lower gallium concentration ($3%), and a 2 : 1 ratio of indium (In) to tin(Sn) in Ag-Galinstan. Therefore, the Ag and Au nanomaterials facilitate two electron transfer processes between BH 4À and MB + , thereby enhancing the electron capacity of the catalyst. Tang et al. prepared a Ga-Pt liquid metal catalyst containing Pt nanoparticles dissolved in Ga to test the catalytic activity in comparison to the commercial Pt/C catalyst in MB degradation. Ga-Pt catalyst is approximately 84 times more active than commercial Pt/C catalyst. Moreover, based on the ratio of surface Pt atoms in Ga-Pt and Pt/C (Ga-Pt : Pt/C ¼ $8.6 Â 10 À5 ), it is estimated that the activity of Pt atoms in the Ga-Pt system is more than ve orders of magnitude greater than that of Pt/C. Liang et al. 78 proposed a liquid metal/metal oxide core-shell heterostructure catalyst. The liquid metal was chemically modied with Cu/W/Mo/Ni metal nanoparticles forming Ga 2 O 3 core-shell heterostructure catalysts and applied to photocatalytic degradation of organic pollutant (methylene blue and congo red) stock solution. The degradation of methylene blue and congo red by Ni-LM catalyst was found to be 92% and 79%, respectively ( Table 2).

Discussions
The worldwide energy crisis is monumental. To meet the escalating energy demand and develop sustainable energy sources, it is urgent to make revolutionary cost and scalability advancements. Scalability becomes the deciding factor between research and industrial applications in the same phase when designing application-specic processes such as hydrogen  economy and sustainable energy solutions, which must operate on large scales inevitably. Central to scalability considerations is the intersection between cost, large-scale processing, ease of fabrication, and ensuring a stable supply of materials. In summary, Ga-based liquid metal catalysts have relatively low viscosity, which allows the active sites on liquid surface to be regenerated spontaneously with the Ga atoms ow in the liquid, or by designing a bubbler-type reactor with gas bubbles as the driving force for the Ga atoms ow, resulting in far more theoretical active sites than conventional solid catalysts and a signicantly longer catalyst lifetime. As a metal solvent, Gallium, EGaIn or Galinstan are capable of solubilizing almost all noble metals and transition metals, whereas it has been reported that specic metal oxides show a certain solubility in liquid Ga alloys, however, the species of metal oxides that can be solubilized are not clear yet. To ensure the scalability of LM catalysts in energy applications, the selection of metals must be restricted to those that are abundant and inexpensive. In addition, Ga is relatively inexpensive in bulk at absolute atmospheric pressure compared to several solvents for industrial applications, such as ionic liquids, and it is also a relatively abundant element in the earth's crust. Although mercury is a relatively inexpensive metal, its high toxicity clearly prevents it from being utilized. Overall, it is anticipated that the maturity of the metal economy and the excellent recoverability of metal will result in the expansion of LM-catalyzed processes. LMs have been successfully implemented in large commercial processes to date. Consequently, even though LM catalysis is still an emerging eld, operational knowledge from these applications can be applied to the development of scalable breakthroughs in LM catalysis to ensure optimal production levels at low costs. At this stage, the research of liquid metal catalysts focuses primarily on the following aspects: (1) In alkane dehydrogenation, additional modulation of reaction conditions and adjustment of metal components may be attempted to enhance the catalytic performance of various alkane selectivity.
(2) To avoid and reduce the use and even the waste of precious metals, research on methods to recover precious metals from liquid metals and the improvement of catalyst performance should be expanded, thereby preventing the use of various metals in liquid metal alloys.
Catalysts based on liquid metal materials, such as room temperature liquid metal catalysts (EGaIn, Galinstan), bimetallic-liquid metal catalysts, polymetallic-liquid metal catalysts, and liquid metal multiphase catalysts, offer new opportunities for the advancement of catalytic science and engineering and provide new catalytic routes for a wide range of existing industrial catalysis. Among the catalytic reactions for which liquid metal catalysts hold promise is: (1) The metals utilized in cutting-edge metal hydrogen storage technology are typically reactive. Ga and these reactive metals can form an alloy that will protect these metals while preserving their properties, since the surface of liquid Ga can form a dense oxide layer that prevents air and water vapor from reacting further with the metal.
(2) It is unknown whether the products of CO 2 catalytic degradation can be converted into chemicals with added value via hydrogenation or other methods.
(3) It must be determined if additional metals can be added to Ga, EGaIn, and Galinstan to create polymetallic catalysts that can be used for more energy-and environment-friendly catalytic reactions.
(4) The organically polluted wastewater contains a variety of contaminants. It is possible to study the selectivity and catalytic performance of various liquid metals for various organic pollutants, including photocatalysis and electrocatalysis.
(5) SAC in SCALMS as an emerging research highlight await further exploration by researchers, covering fabrication methodologies, component regulation, potential catalytic reaction species and mechanisms that can lead to better performance than bulk metal catalysts.
Briey, previous research on LM catalysts has demonstrated their multidisciplinary potential. Researchers believe that Gabased liquid metal catalysts will soon provide new catalytic routes for a variety of applications, thereby expanding the scope of catalytic chemistry.

Conclusions
This review presents a selection of typical research results on liquid metal catalysts and describes signicant research on the use of liquid metal materials in catalytic applications over the past 15 years. With its low viscosity and liquid properties, the liquid metal enables the catalytic active sites to continuously regenerate, thereby extending the catalyst's lifetime prior to deactivation and making it more resistant to overall catalyst deactivation caused by deactivation of the active sites on the surface of the solid catalyst. In addition to nearly all precious and transition metals having a reasonable solubility in liquid Ga, liquid-gas phase gases also have a certain solubility. Environmental and energy catalysis are the two main application sectors for LM catalysts. Several practical applications are also discussed, including catalysis for the synthesis of ethylene via non-petroleum routes, alkane dehydrogenation, CO 2 hydrogenation to methanol, and catalytic degradation of CO 2 . In addition, a summary of the various performance evaluations of Pd, Pt, and Ni alloys with Ga/Ga oxides, EGaIn/Galinstan with Au and Ag under multiple metal components and reaction conditions is provided. It has been demonstrated that liquid metal catalysts play an important role in enhancing the efficiency of chemical reactions and can be utilized in a variety of elds, and signicant progress has been made. However, research on liquid metal catalysts is still in its infancy, and challenges such as how to form different metal types with different catalytic activities on the surface of liquid metal and the application of liquid metal catalysts in a variety of elds are yet to be resolved.

Conflicts of interest
There are no conicts to declare.